BUBBLE RUPTURE IN BUBBLE ... Chen, R., et al.: Bubble Rupture in Bubble Electrospinning THERMAL...
Embed Size (px)
Transcript of BUBBLE RUPTURE IN BUBBLE ... Chen, R., et al.: Bubble Rupture in Bubble Electrospinning THERMAL...
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149 1141
BUBBLE RUPTURE IN BUBBLE ELECTROSPINNING
Rouxi CHEN a,b, Yuqin WAN d, Na SI c, Ji-Huan HE a,b*, Frank KO d, and Shu-Qiang WANG e*
a National Engineering Laboratory for Modern Silk, College of Textile and Clothing Engineering, Soochow University, Suzhou, China
b Nantong Textile Institute of Soochow University, Nantong, China c Nantong Bubbfil Nanotechnology Company Limited, Nantong, China
d Department of Material Engineering, University of British Colombia, Vancouver, Canada e Research Center for High Performance Computing, Shenzhen Institutes of Advanced Technology,
Chinese Academy of Sciences, Shenzhen, China
Review paper DOI: 10.2298/TSCI1504141C
As the distinctive properties and different applications of nanofibers, the demand of nanofibers increased sharply in recently years. Bubble electrospinning is one of the most effective and industrialized methods for nanofiber production. To op- timize the set-up of bubble electrospinning and improve its mass production, the dynamic properties of un-charged and charged bubbles are studied experimental- ly, the growth and rupture process of a bubble are also discussed in this paper. Key words: bubble electrospinning, bubbfil spinning, dynamic of bubble,
growth and rupture of bubble, nanofiber, mass production
Nanofibers have been extensively explored in last decades ; their distinctive properties (high surface area in combination with different functionalities) make them one of the most promising candidates in diverse areas , such as filter, tissue engineering, drug de- livery, protective clothing, advanced biomaterials, biosensors, etc.
Conventional single-needle electrospinning is a simple, effective, versatile, cost- effective method to produce polymer nanofibers. However, it has a small fiber production rate, typically less than 0.3 g per hour per needle , which greatly limits its practical applica- tions in industrial and civil products. Recently the needle-less (free liquid surface) electrospinning technology have been reported as new viable possibilities to fabricate nanofibers in mass production . Hundreds of labs and research institutions have attempted to find new methods to improve the production of nanofibers.
Bubble electrospinning is one of the most influential needle-less electrospinning methods, and it has been developed into a matured bubbfil spinning . Inspired by the fantas- tic spider spinning, Liu and He  and Liu et al.  used a gas pump to generate bubbles on a polymer liquid surface which was charged with an electric voltage, a number of jets were gen- erated from the surface of the bubbles. They also applied “theory of bubble dynamics” to ex- plain the mechanism of mass nanofiber production [8, 9]. In a number of publications, efforts have been described in finding the controlling parameters for different polymers using bubble –––––––––––––– * Corresponding authors; e-mails: firstname.lastname@example.org, email@example.com
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning 1142 THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149
electrospinning. Yang et al.  investigated the effects of solution concentration and viscosity on the diameter and morphology of bubble electrospun polyvinyl alcohol (PVA) nanofibers. Kong et al.  suggested a new method for fabrication of nanofibers with a polymer bubble membrane, and studied the effects of applied voltage and collect distance on the fiber diameter. Gule et al.  used bubble electrospinning to prepare DMHF-containing PVA nanofibers, which demonstrated good antimicrobial and cell-adhesion inhibition efficiency. Dou et al.  investigated the morphology of nylon6/66 nanofibers yarns produced by bubble-spinning. Chen et al. fabricated crimped nanofibers by bubble electrospinning and explored its crimp mecha- nism . The authors also described the surface tension of a bubble with a modified Young- Laplace equation , which can be widely applied for bubble spinning process analysis. Li et al.  studied the effect of airflow direction blowing on polymer bubble and the morphology difference of the superfine fibers. Li et al.  compared the fiber morphologies of polyether sulfone (PES) via bubble spinning vs. conventional single needle electrospinning under the same spinning conditions. Shen et al.  prepared multi-layer nanofiber nonwoven fabrics for PM2.5 mask, which admitted excellent filter capabilities and breathability. Sidaravicius et al.  fabricated PEO/PVA nanofibers using a bubble foamed polymer solution to promote high mass deposition and investigate its deposited intensity. Ren et al.  used the foaming-assisted electrospinning technique to get large-pore mesoporous ZnO nanofibers. Jiang et al.  demonstrated an improved approach of free surface electrospinning utilizing micro-bubble solu- tion system and studied the effect of bubble size on the diameters of nanofibers. Figure 1 shows different nanofiber morphologies of different polymer via bubble electrospinning.
(a) (b) (c)
(d) (e) (f) Figure 1. The scanning electron microscopy of the nanofiber membrane via bubble spinning set-ups; (a) PVA (DI water) nanofiber, (b) PES (DMF) nanofiber, (c) PLA(DMF) nanofiber, (d) PES (DMF) nanopore fibers; (e) nylon (formic acid) nanofibers; (f) PS(THF) nanofibers
These researches mainly focused on the preparation and application of various poly- mer nanofibers via bubble electrospinning, but fewer literature reported the dynamical mecha- nism of bubble forming and its application in electro-spinning for mass production of nanofibers. In view of this, in this paper, the growth situation and rupture process of un-charged and charged polymer bubble were discussed, which further explained the reasons why bubble electrospinning will be one of the most effective methods for mass production of nanofiber.
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149 1143
Materials: PVA, with an average molecular weight of 95,000 g/mol purchased from Aladdin, sodium dodecyl benzene sulfonate (SDBS) purchased from Sinopharm Chemical Reagent Co., Ltd, and deionized water were used in these experiments. All materials used without further purification.
Solution preparation: PVA particles and SDBS powder were dissolved into DI water at the room temperature. The mixture was then placed on a 120 °C heating plate and stirred until a homogeneous and transparent solution was obtained. The solution was then cooled down to room temperature for experiment. The concentration of PVA solution was 6 wt.%.
Electrospinning set-up: fig. 2 shows the schematic of a classical bubble spinning set-up, which includes a bubble generator, a spinneret, an air pump, a solution reservoir, a high-voltage pow- er supply, and a grounded collector. The grounded collector was placed 20 cm upper to the spinneret.
The forming and vanishing process of un- charged and charged polymer bubbles were respec- tively recorded with a high speed camera (HSC). The photos were further dissected to investigate the growth and rupture process of bubble.
During the experimental process, to begin with, the air pump was switched on until the gen- erated bubbles were continuously pumped into the spinneret; the growth and rupture process of the un-charged bubble was videoed. And then, the ap- plied voltage was applied and increased until a number of jets were observed from the top of the spinneret, the movement of the charged bubbles was also videoed. The experiments were carried out at room temperature in the air.
Shown as fig. 1, nanofibres with various morphologies, such as smooth, nanoporous, micro-spherical with nanoporous, can be fabricated. The key to a successful bubble electrosping is the steady continuous generation and rupture of polymer bubbles.
The nanofiber formation and the obtained nanofiber properties in bubble electrospinning depend on polymer solution properties including viscosity, solution concen- tration, surface tension and electrical conductivity.
Young-Laplace equation When an air bubble generates from the surface of a polymer solution, the force
pushing it upward can be expressed in the form:
2upward in out( )πF P P R= − (1)
where Pin is the inner pressure of the bubble，Pout – the out pressure of the bubble, and R – the radius of the bubble. The gravitation could be ignored as the mass of bubble is extremely low.
The downward force of bubble, related with the surface tension of polymer solution, can be expressed in the form:
Figure 2. The schematic of a classical bubble spinning set-up
Chen, R., et al.: Bubble Rupture in Bubble Electrospinning 1144 THERMAL SCIENCE, Year 2015, Vol. 19, No. 4, pp. 1141-1149
downward 2πF Rγ= (2)
where γ is the surface tension of polymer solution. Since
upward downwardF F= (3)
it`s surface tension T can be expressed in the form :
in out 1 ( ) 2
T R P P= − (4)
When the bubble has an aspheric surface, the inner radius of the bubble can be ex- pressed as R1 and R2, according to the Laplace equation, it`s surface tension T can be also ex- pressed in the form:
1 1 P P